domain: phys chim

text:
Dynamic HAADF STEM observation of single atom chain as transient state of Au ultrathin nanowire breakdown.

Lise-Marie Lacroix, † * Raul Arenal, ‡+ * Guillaume Viau † . † LPCNO, Université de Toulouse, INSA, UPS, LPCNO (Laboratoire de Physique et Chimie des Nano-Objets), F-31077 Toulouse, France; CNRS; UMR 5215 ; LPCNO, F-31077 Toulouse, France ‡ Laboratorio de Microscopias Avanzadas (LMA), Instituto de Nanociencia de Aragon (INA), U. Zaragoza, C/ Mariano Esquillor s/n, 50018 Zaragoza (Spain). + Fundacion ARAID, 50004 Zaragoza, Spain.

Supporting Information Placeholder

ABSTRACT: Ultrathin chemically grown Au nanowires undergo irremediable structural modification under external stimuli. Thanks to dynamic high-angle annular dark field imaging, electron beam induced damaging was followed, revealing the formation of linear gold atom chains as long as reactive clusters on the side, opening fascinating perspectives for both catalysis and electronic transport applications.

Metallic nanowires represent ideal objects for fundamental studies as long as potential applications in sensing, 1 catalysis and electronic contacts. 2,3 Quantized conductance scaling with 2e 2 /h was observed in atomic wires obtained by mechanical deformation of point contact, 4,5,6 breaking junction, 7 electrochemical approaches. 8 Recently, ultrathin gold nanowires exhibiting a diameter of 1.7 nm and a micrometric length were synthesized by reduction of gold chloride salt in presence of oleylamine. 9,10,11,12 These highly crystalline wires, grown along the <111> direction of the fcc structure, opens great perspective for electronic transport studies. 13,14 Their small diameter leads to quantized phenomena while their extreme aspect ratio render physical contact by lithography feasible. 14,15 However, thin metal nanowires are prone to fragment into chain of spheres at high temperature, as described by the Plateau-Rayleigh instability. 16,17 The critical temperature at which this phenomenon occurs is strongly dependent on the wire surface energy and thus on the crystalline surface exposed and on the ligands adsorbed. 18 Other perturbation such as electron beam can also induce such instability. 19 Radiolysis, due to plasmon losses, and knock-on damage, resulting from high energy scattering, are the two most common types of primary damage that occur in irradiated samples, 20 depending on their electronic state. 21,22 We report here for the first time a dynamic study of the Au wire breaking by HAADF-STEM. Sub atomic resolution obtained with the aberration corrected microscope combined with the high diffusion of Au enabled to follow the trajectory of individual atoms, evidencing the formation of atom chains prior to the breaking and free clusters aside. 1.7 nm ultrathin Au nanowires were obtained in liquid phase following previously reported synthesis (Figure 1a). The Z-contrast nature of HAADF-STEM imaging makes this technique an ideal method for identifying heavy atoms (as gold, Z=79) on light supports (carbon, Z=6, in the present case) as evidenced in Figure 1b. Surprisingly, at 80 kV and under very low dose (0.0145 e -A -2 s -1

), the degradation of Au NWs was extremely fast (Video S1-S2). However, at 300 kV, the electron beam damaging could be dynamically followed using a 1.6 frame.s -1 scanning (Video S3-S9). It is well established that higher accelerating voltage reduces radiolysis damage due to lower inelastic scattering probability. However, opposite happens for knock-on damage, the threshold for gold clusters and particles being above 200 and 400 kV respectively. 24,25 As a consequence, though gold is a good conductor, the evolution of these Au NW seems to be governed by radiolysis at low voltage. At 300 kV, atomic columns as long as individual atoms on the side of the wire could be detected as evidenced in Figure 1b. The wire breaking occurred through a continual structural reorganization, with multiple twin boundaries, as long as a thickening of the initial diameter, leading to rough surfaces, as evidenced in Figure 2 and supplementary videos S1.

Contrarily to the theoretical model of Plateau Rayleigh instability, 26 the breakdown involves first an asymetric modification of the apexes. Moreover, prior to disruption, two types of chains were observed exhibiting 3-4 atoms (Video S3-S6 and Figure S1) or single-atom thickness (Video S3, S7-S8, Figure 2a-b andS2). The single-atom chains (SAC) results from the downsizing of the channel from 3-4 atoms down to a single one as evidenced by the successive snapshots in Figure 2a-b extracted from video S3. On the contrary, some multi-atom chains (MAC) exhibit a different behavior and break very suddenly (Figure S3). These two types were previously reported on gold nanowires obtained by HRTEM irradiation of a Au polycrystalline thin film. 27 Due to the constant rotation of the wire under the electron beam, the atomic positions could not always be resolved. We followed two cases of single atom chain (SAC) and multi atom chain (MAC) breaking, for which the wire stays in zone axis. In the case of SAC formation (Figure S4), the wire remained highly crystalline along the <111> direction, with a continuity of the dense plane across the junction. If twin planes are mobile, as previously reported, 28,29 the apexes only rotates of few degrees (~2°) respectively to each other (Figure S4). SAC exhibit an important flexibility as evidenced by the drastic modification of its inclination, likely due to the mobility of the anchoring atoms. 30 The interatomic distance within atom chains was found in the range 0.23 -0.31 nm, with a median at 0.29 ± 0.10 nm, in agreement with the nearest-neighbor distance in gold (0.29 nm). 30 The larger interatomic distance of 0.31 nm, may result from the carbon contamination as previously reported. 31 In the case of MAC (Figure S5), important recrystallization occurred. Contrarily to SAC, the dense planes are highly tilted, resulting in apex direction rotated of 23° respectively to the <111> direction. The position of atoms in the MAC, was analyzed and revealed unambiguously a portion of dense plane (60° angles) with slight positional disorder (Figure S5). The interatomic distance was found in the range 0.24 -0.29. Contrarily to the previous reports, the observed MAC is only one atom thick and do not exhibit helical multi-shell structure. 32 Concomitantly to the chain formation, individual Au atoms were steadily ejected and migrate from the shrinking channel. The trajectory of each atom could be followed, evidencing the formation of small clusters such as dimers or trimers. These clusters were fairly unstable and could dissociate after few seconds to yield isolated atoms. Such metallic clusters have been reported as highly reactive for catalysis, and in the case of gold, towards CO oxidation. 33,34 Combined with the presence of the highly twinned and rough Au wires, 35 enhanced catalytic activities are expected. Formation of quantized atomic channel along the wire length is clearly evidenced during the fragmentation process. These intermediate states were stable enough to be imaged at 300 kV for few seconds. Modification of the wire surface energy, through ligands exchange process, could enable to further stabilize the single-atom thick chains, 8 , 36 and thus open great perspective for the easy-made parallel quantized wires. Appearance of small and highly reactive clusters strengthens the potentiality of ultrathin Au nanowire for catalysis. Though studied under electron beam irradiation, similar breaking mechanism, involving channel shrinking and ejection of reactive atoms may occur under any external stimuli such as current flow or temperature rising, commonly used for Rayleigh instability studies.

ASSOCIATED CONTENT

Supporting Information

Experimental details and videos are available free of charge via the Internet at http://pubs.acs.org.

Table of Content

  23Briefly, a 10 mM HAuCl4 solution was reduced by triisopropylsilane in presence of oleylamine at 40°C for 1h30. The reducing agent and surfactant excess was removed by purification prior to the deposition of Au wires on the carbon coated Cu grid. Electron-beam shower, during 20-25 min, was performed in-situ to prevent contamination during STEM experiments. HAADF-STEM study was performed with an aberration corrected microscope working at 80 -300 kV. The aberration-free probe is taken to have a 25 mrad converge semi-angle, providing a resolution of ~1.3 Å (80 kV) and ~0.8 Å (300 kV). The inner and outer collection angles used in recording the HAADF images were 60 and 200 mrad, respectively. Low electron doses of 0.0145 e -300 kV) were employed.

Figure 1 .

 1 Figure 1. a) TEM and b) HAADF-STEM images of Au nanowires.

Figure 2 .

 2 Figure 2. Snapshots extracted from video S3 of E-beam induced wire breaking which proceeds through the decrease of the channel diameter from a) 3 atoms to b) single atom. c) resulting 7 nm rods surrounded by Au atoms and dimers. As insets, schematic 3D views of a) MATC, b) SATC and c) dimer and isolated atoms. Scale bar : 1 nm. White arrows indicate twin planes

  Rodrigues et al. invoked the difference of crystalline orientation of the atom chains obtained, [110] versus [111] or [100] respectively, to explain such discrepancy. Starting from single-crystalline Au nanowires grown along <111> direction, we did not expect such variety.

AUTHOR INFORMATION

Corresponding Author

Lise-Marie Lacroix. lmlacroi@insa-toulouse.fr. Tel : +33567048833.Fax : +33561559697 Raul Arenal, arenal@unizar.es, Tel : +34976762985

Author Contributions

All the authors contributed equally.

Notes

The authors declare no competing financial interests.

ACKNOWLEDGMENT

The authors acknowledge the financial support of the Labex NEXT, N° 11 LABX 075, and of the European Associated Laboratory LEA TALEM. The scanning transmission electron microscopy studies were conducted at the Laboratorio de MicroscopiasAvanzadas (LMA) at the Instituto de Nanociencia de Aragon (INA) -Universidad de Zaragoza (Spain). The TEM measurements were supported by the European Union Seventh Framework Program under Grant Agreement 312483 -ESTEEM2 (Integrated Infrastructure Initiative -I3).


domain: chim phys sdv.can

text:
Lise-Marie Lacroix

Fabien Delpech

Céline Nayral

Sébastien Lachaize

Bruno Chaudret

New generation of magnetic and luminescent nanoparticles for in-vivo real-time imaging

Keywords: Contrast agents, MRI, Near-Infra Red, luminescent nanocrystals, quantum dots, core-shell

A new generation of optimized contrast agents is emerging, based on metallic nanoparticles (NPs) and semiconductor nanocrystals (NCs) for respectively magnetic resonant imaging (MRI) and near-infra-red (NIR) fluorescent imaging techniques. Compared with established contrast agents such as iron oxide NPs or organic dyes, these NPs benefit from several advantages: their magnetic and optical properties can be tuned through size, shape and composition engineering, their efficiency can excess by several order of magnitude that one of contrast agents clinically used, their surface can be modified to incorporate specific targeting agents and antifolding polymers to increase the blood circulation time and the tumor recognition, they can possibly be integrated in complex architecture to yield multimodal imaging agents. In this review, we will report the materials of choice based on the understanding of the physics basics of NIR and MRI techniques and their corresponding syntheses as NPs. Surface engineering, water transfer, and specific targeting will be highlighted prior to their first use for in-vivo real-time imaging. Highly efficient NPs, safer in use and target specific are likely to be entering clinical applications in a near future.

Since the discovery, by chance, of X-ray potentiality by Roentgen in 1896, imaging techniques have been optimized and extended. Depending on the penetration depth, the spatial resolution and the sensitivity required, X-ray computed tomography (CT), Positron Emission Tomography (PET), Magnetic Resonance Imaging (MRI) or optical imaging, such as Near-Infrared (NIR) fluorescent imaging, may be selected as the most relevant imaging modality [START_REF] Cassidy | Molecular imaging perspectives[END_REF]. In all cases, enhancement of the signal over noise ratio, and thus of the sensitivity of these imaging techniques, requires the introduction of contrast agents such as radioisotopes, paramagnetic molecules or more recently inorganic nanoparticles [START_REF] Cho | Inorganic nanoparticle-based contrast agents for moleuclar imaging[END_REF]. The latter have benefited from tremendous advances during the last two decades notably in terms of available synthetic routes. In particular, the improvements of the solution-phase approaches allow now an easy and low-cost access (compared to classical physical or vacuum methods) to wellcontrolled nano-probes. Prominent examples of imaging modalities which have profited from this intense research activity are MRI and NIR luminescence: a new generation of sophisticated nano-objects has reached such stage of maturity, especially in terms of probe sensitivity, that their use has on one hand, become a standard practice in in vitro biology research and on the other hand, hold promise for in-vivo real-time detection. This review intends to highlight these advances and developments that occurred in the last few years for MRI and NIR luminescence detection. In the case of MRI, the upgrading of contrast agents based on oxide NPs to metallic NPs yields to strongly enhanced probe sensitivity. As will be detailed herein, this was achieved thanks (i) to the unprecedented magnetization related on metallic nature of the NPs and (ii) to the narrow size distribution allowing homogeneous and intense magnetic properties from one NP to another. Similarly, in the case of NIR, impressive progress has been realized on the synthesis of quantum dots (QDs) able to absorb and emit efficiently in the NIR range of wavelength (where the transmissivity of organic tissue is maximum). Additionally, following the trend toward "greener" chemistry, new versions of QDs free of Cd, Pb and Hg are now available. These significant advances have motivated this review dedicated to an up-to-date perspective on magnetic NPs and NIR emitting QDs. Moreover, because of different features in terms of sensitivity, resolution, acquisition time and operational costs, fluorescence-based in vivo imaging techniques are complementary to MRI. [START_REF] Cassidy | Molecular imaging perspectives[END_REF] NIR enables faster measurements with higher sensitivity. [1, 3 , 4 ] while MRI ensures a higher spatial resolution and depth of penetration. Thus, very recent work focused on bimodal NPs, i.e. combining MRI and NIR modalities, will also be addressed as challenging perspective in view of designing more and more sensitive probes and/or multifunctional theranostic nano-objects (MRI contrast agents can also be used as heating centers in magnetic hyperthermia). [START_REF] Lacroix | Recent advances in Magnetic Nanoparticles for Diagnostic and Therapeutic Applications[END_REF] After a general introduction on liquid phase synthesis of NPs, we will present the basics of MRI and the general chemical synthesis for new generation of optimized contrast agents. Near infra-red fluorescence technique requirements will then be discussed, optimal material being highlighted. Corresponding type-I and type-II quantum dots synthesis will be listed. MRI and NIR contrast agents being prepared mostly in organic solvants, we will review the surface engineering strategies to ensure the water-transfer of generic inorganic NPs and their further biodistribution and specific targeting. Up-to-date results of real time in-vivo MRI and NIR imaging obtained with new generation of NPs will be reviewed before concluding on the requirements and first promising attempt for NIR/MRI multifunctional NPs.

I. Liquid-phase synthesis of inorganic NPs

This brief part aims at introducing the general principles of NPs synthesis in solution to

give the reader the keys to a deep understanding of the numerous synthesis examples presented hereafter (parts II.2 and III.2). This review focuses on the chemical approach to NPs formation particularly because of its ability to provide NPs samples (i) of high quality and (ii) in adequate amounts for further biological use.

Colloidal solutions of nanoparticles of various natures (metallic, semi-conducting, oxides) can be prepared by chemical approach. The general strategy followed relies on the decomposition of a precursor, typically a salt or an organometallic compound (Figure 1). This decomposition yield free atoms which tend to aggregate to form small seeds during the nucleation step. Metallic NP synthesis may require the use of a reducing agent to convert oxidized atoms (M n+ ) into metallic atoms (M 0 ). The seeds formed during the nucleation step then grow by successive addition of atoms, by coalescence or through a ripening based process [ 6 , 7 ]. To prevent NPs from aggregation and sintering, organic molecules (surfactants) or polymers are added to ensure steric hindrance or electrostatic repulsion between NPs.

Figure 1. Schematic view of the general mechanism driving chemical NP synthesis.

Since physical properties depend on the size, size distribution and shape of NPs, nucleation and growth steps must be carefully tuned. Monodisperse NPs (with a narrow size distribution σ < 10%) could be prepared via a burst nucleation, fast and limited in time, followed by a homogeneous growth [START_REF] Park | Synthesis of monodisperse spherical nanocrystals[END_REF]. Nucleation and growth steps extent depends of experimental parameters such as reaction time, temperature, nature of the precursors and surfactants, thus careful optimization of these parameters are usually required. [START_REF] Shevchenko | Study of nucleation and growth in the organometallic synthesis of magnetic alloy nanocrystals : the role of nucleation rate in size control of CoPt 3 nanocrystals[END_REF] II. MRI principle and nanomaterials:

In this section we will first introduce the basics of MRI, highlighting the requirements for optimized contrast agents : (i) high magnetization materials, (ii) large magnetic core size, and

(iii) core accessibility to water protons. Up-to-date syntheses of magnetic nanoparticles will then be reviewed in the context of in vivo MRI imaging i.e. (i) metallic material preferred to oxides due to their enhanced magnetization and (ii) narrow-size distribution to ensure homogeneity of the magnetic properties.

II.1 Basics of MRI:

Clinical MRI is based on the relaxation of the nuclear spin of water protons in a strong magnetic field (1.5T to 3T in hospitals, 9T or greater in laboratories). Into such static field B 0 , spins tend to align parallel or antiparallel (Figure 2a), and precess at the Larmor frequency ω 0 which is propotional to the field strength:

ω 0 = B 0 .γ (Eq. 1)
where γ is the gyromagnetic ratio (for hydrogen, γ = 42,6 MHz/T) Once magnetized by the static field, protons can be excited through a perpendicular pulsed field B 1 (rotating around the B 0 axis at the Larmor frequency, i.e. in the radio frequency range RF), which leads to a magnetization M xy that is perpendicularly to B 0 (Figure 2b). After the removal of the RF field, spins tend to realign with B 0 following (Figure 2): a longitudinal relaxation (M Z increasing according to an exponential law, time constant T 1, Figure 2d), and a transverse relaxation (exponential decay of M xy , time constant T 2, Figure 2e). MR images are acquired while protons return to their equilibrium state, contrast being based on the difference of relaxation rate R i =1/T i (i=1 or 2). Relaxation rate depends of numerous parameters among which the surrounding medium, field strength, temperature, accessibility of protons and of course nature of the contrast agents. Intrinsiquelly, tumor cells exhibit different relaxation constants compared to healthy surrounding tissues, which can lead to an MRI contrast. However, dedicated cancer imaging may require an enhancement of the signal over noise ratio.

Static magnetic field applied can be increased to accelerate the precession of spins (Eq.

1) and to slightly improve the excess proportion of spins aligned parallel (low energy state).

Signal being linked with the relative magnetization of tissues, i.e. the spin excess, enhancement could be reached. However, establishing large homogeneous field on whole body is not technologically easy, thus improvement of signal at fixed magnetic field strength (up to 3T), through the introduction of adequate contrast agents, is still required.

Paramagnetic, superparamagnetic or ferromagnetic contrast agents affect both relaxation processes [START_REF] Lin | Magnetic nanoparticles for early detection of cancer by magnetic resonance imaging[END_REF]. However, depending of their nature, they will increase more specifically the relaxation rate R 1 (positive contrast agent) or R 2 (negative contrast agent).

Paramagnetic ions (mainly Gadolinium(III) complexes) have been widely used as positive contrast agents in clinical applications. [START_REF] Caravan | Gadolinium(III) chelates as MRI contrast agents : structure, dynamics and applications[END_REF][START_REF] Caravan | Strategies for increasing the sensitivity of gadolinium based MRI contrast agents[END_REF][START_REF] Leon-Rodriguez | Responsive MRI agents for sensing metabolism in vivo[END_REF] However, high dose of these toxic metal ions are required due to the relatively low efficiency of Gd-based contrast agents.

Nanoparticles, among which iron oxides NPs, have received lots of interest as efficient non toxic R 2 contrast agents for the last 20 years. [START_REF] Na | Inorganic nanoparticles for MRI contrast agents[END_REF] Magnetic nanoparticles are small magnets which generate a magnetic field at their vicinity (Figure 3). Such field inhomogeneity accelerates the phase decoherence of the spins [START_REF] Cheon | Synergistically integrated nanoparticles as multimodal probes for nanobiotechnology[END_REF]. Therefore, NPs act as negative contrast agents, their efficiency being quantified through the normalized relaxativity r 2 =R 2 /concentration (mMol -1 s -1 ). In first approximation, relaxativity varies as the square of the magnetic field induced at the vicinity of the water proton. The magnetic field is a short-distance perturbation, which vanishes quickly:

r α d -6 .(M S V) 2 (Eq. 2)
where d is the distance proton-center of the magnetic NP, M S is the saturation magnetization and V the volume. The accessibility of the water proton to the NP surface is of particular importance due to the d -6 decrease of r. Therefore, from a magnetic point of view, the coating of magnetic core, which ensure the biostability of the inorganic NPs as described in section 3, should be as thin as possible to yield high relaxativity (Table 1). However, biostability often requires relatively large coating, as discussed in section 3, thus, a delicate balance should be found regarding the corona shell thickness.

In order to improve the relaxativity, larger NPs could also be used [START_REF] Tromsdorf | Size and surface effects on the MRI relaxativity of manganese ferrite nanoparticle contrast agents[END_REF][START_REF] Lee | Waterdispersible ferromagnetic iron oxide nanocubes with extremely high r2 relaxativity for highly sensitive in vivo MRI of tumors[END_REF] (Table 1), but size affects the magnetic behaviour of nanoparticles. At small size (below 12 nm for Fe), NPs behave as paramagnetic species (superparamagnetism): they can be easily magnetized under B 0 and do not exhibit magnetization in absence of magnetic field (remnant state Mr=0).

At larger size, NPs are ferromagnetic and exhibit a net magnetization (Mr≠ 0). This difference of behaviour affects the stability of NPs in solution through the modification of dipolar interactions (in first approximation α Mr 2 [START_REF] Lee | Effect of interparticle interactions and size dispersión in magnetic nanoparticle assemblies : a static and dynamic study[END_REF]). Aggregation of the ferrofluid may arise for ferromagnetic NPs, thus, superparamagnetic NPs have been prevailing materials so far for in vivo applications. Recently, larger NPs with peculiar magnetic configuration (vortex state), have been proposed for bioapplications [START_REF] Yang | Stable vortex magnetite nanorings colloid: micromagnetic simulation and experimental demonstration[END_REF]. These NPs exhibit a very low magnetization in absence of any applied field (weak Mr), resulting in weak interparticle interactions, but a large volume and thus a presumably high relaxativity. Such vortex states are observed for intermediate size range, typically 30 -100 nm for iron [START_REF] Snoeck | Magnetic configurations of 30nm Iron Nanocubes Studied by Electron Holography[END_REF][START_REF] Lacroix | Stabilization vortices in interacting nano-objects : a chemical approach[END_REF].

In addition to the size control, one could optimize M S . Saturation magnetization is an intrinsic parameter of the material chosen and corresponds to the maximum magnetic moment that can be reached upon an applied field. Magnetic dopants, such as Mn, can be added to ferrite materials, leading to a slight increase of M S (Table 1). To further enhance M S , metals, such as Fe or Co, should be preferred to their oxide counterparts (Table 1). Though contrast agents used clinically are nowadays only based on SPION (superparamagnetic iron oxide nanoparticles) [START_REF] Yang | Emerging inorganic nanomaterials for pancreatic cancer diagnosis and treatment[END_REF], the design of optimized contrast agents would benefit from metallic NPs, providing that these NPs do not exhibit toxicity [START_REF] Huang | Biochemical and biomedical applications of multifunctional magnetic nanoparticles : a review[END_REF]. Thus, we will focus our discussion on the recent strategies developed to synthesize and protect metallic nanoparticles with optimized properties. [START_REF] Huang | Facile and green synthesis of biocompatible and bioconjugatable magnetite nanofluids for high-resolution T2 MRI contrast agents[END_REF] or in organic solvents. [START_REF] Laurent | Magnetic iron oxide nanoparticles: synthesis, stabilization, vectorization, physicochemical characterizations, and biological applications[END_REF] Size control could be reached by the decomposition of organometallic precursors at high temperature in presence of long alkyl chain surfactants [START_REF] Park | One-Nanometer-Scale Size-Controlled Synthesis of Monodisperse Magnetic Iron Oxide Nanoparticles[END_REF][START_REF] Sun | Size-controlled synthesis of magnetite nanoparticles[END_REF], further synthesis information being found in recent review articles. [START_REF] Reddy | Magnetic nanoparticles : design and characterization, toxicity and biocompatibility, pharmaceutical and biomedical applications[END_REF][START_REF] Lee | Designed synthesis of uniformly sized iron oxide nanoparticles for efficient magnetic resonance imaging contrast agents[END_REF] Concerning magnetic dopants, they can be added in the spinel structure by co-reduction at high temperature of organometallic precursors such as Mn(acac) 2 and Fe(acac) 3 . [START_REF] Sun | Monodisperse MFe2O4 (M= Fe, Co, Mn) nanoparticles[END_REF] Here, we will focus our attention on synthesis of metallic NPs, promising higher magnetization, as explained previously. Iron being highly reactive towards oxidation, metallic Fe NPs were mainly prepared in organic solvents (Table 2) [START_REF] Huber | Synthesis, properties, and applications of iron nanoparticles[END_REF]. Classicaly, Fe(CO) 5 was decomposed at high temperature in presence of long-chain amine [START_REF] Yang | Facile large-scale synthesis of monodisperse Fe nanoparticles by modest-temperature decomposition of iron carbonyl[END_REF][START_REF] Farrell | Preparation and Characterization of Monodisperse Fe Nanoparticles[END_REF]. Though highly toxic, this precursor benefited from Fe atoms already reduced (oxidation degree 0), therefore no reducing agent were required. However, the magnetic properties of the NPs obtained were generally lower than the bulk value, due to their intrinsic carburation from CO byproduct [START_REF] Meffre | A simple chemical route toward monodisperse iron carbide nanoparticles displaying tunable magnetic and unprecedented hyperthermia properties[END_REF].

Material

To prevent such carburation, Fe(CO) 5 can be replaced by iron salts or organometallic compounds whose decomposition did not yield any carbon source. Due to their high stability, the decomposition and reduction of iron salts required harsh conditions. For instance, FeCl 2 could be reduced in water by sodium borohydride, but boron contamination has been found to decrease the NP moment [START_REF] Hadjipanayis | Metallic Iron Nanoparticles for MRI Contrast Enhancement and Local Hyperthermia[END_REF]. Therefore, decomposition of organometallic compounds such as Fe(C 5 H 5 )(C 6 H 7 ) [START_REF] Cheong | Simple synthesis and functionalization of iron nanoparticles for magnetic resonance imaging[END_REF] or {Fe[N(SiMe 3 ) 2 ] 2 } 2 [START_REF] Dumestre | Superlattices of iron nanocubes synthesized from Fe[N(SiMe3)2]2[END_REF][START_REF] Lacroix | Iron nanoparticle growth in organic superstructures[END_REF] under dihydrogen atmosphere could be preferred to yield unoxidized iron NPs in mild conditions (bulk magnetization). Due to its high reactivity, the latter amido precursor could also be reduced solely by a long chain amine in absence of H 2 [START_REF] Meffre | Use of long chain amine as a reducing agent for the synthesis of high quality monodisperse iron(0) nanoparticles[END_REF]. The optimization of the nucleation and growth steps, through the tuning of experimental parameters (temperature, surfactants), yielded Fe NPs with unprecedent size and shape control in the range 1 to 100 nm (Figure 4a-b).

Cobalt NPs can be prepared following similar procedures. Co 2 (CO) 8 could be decomposed at high temperature to yield monodisperse NPs [START_REF] Puntes | Colloidal nanocrystal shape and size control : the case of cobalto[END_REF][START_REF] Keng | Synthesis and self assembly of polymer-coated ferromagnetic nanoparticles[END_REF]. As observed for Fe, the binding of -CO species at the NPs' surface decreased their magnetic properties [START_REF] Osuna | Synthesis, characterization, and magnetic properties of cobalt nanoparticles from an organometallic precursor[END_REF]. Cobalt salt (CoCl 2 ) could be reduced with strong reducing agent (superhydride LiEt 3 BH) but yield NPs with ε-Co crystalline phase with degraded magnetic properties prior to annealing treatment [START_REF] Sun | Synthesis of monodisperse cobalt nanocrystals and their assembly into magnetic superlattices[END_REF]. Co can crystallize in hexagonal compact (hcp) structure which exhibit optimized magnetic properties. Benefiting from the crystallographic unicity of the c axis, intensive researches have been devoted to the synthesis of anisotropic Co NPs. Polyol synthesis [START_REF] Soumare | Kinetically controlled synthesis of hexagonally close-packed cobalt nanorods with high magnetic coercivity[END_REF] as long as organometallic approaches [START_REF] Dumestre | Unprecedented crystalline super-lattices of monodisperse cobalt nanorods[END_REF][START_REF] Liakakos | The big impact of a small detail : cobalt nanocrystal polymorphism as a result of precursor addition rate during stock solution preparation[END_REF] yielded single crystalline Co nanorods with a relatively narrow size distribution (Figure 4c). Though nanorods have never been tested for MRI purposes, they could potentially present high relaxativity, analogously to elongated Co@Au nanowonton, prepared through physical process [START_REF] Bouchard | Picomolar sensitivity MRI and photoacoustic imaging of cobalt nanoparticles[END_REF]. (Table 1) compared to iron oxides (125 emu/g FePt [START_REF] Sun | Recent Advances in Chemical Synthesis, Self-Assembly, and Applications of FePt Nanoparticles[END_REF]) and a high cytotoxicity, making them potent anticancer drug due to the leaching of Pt ions in biological condition. [START_REF] Gao | Multifunctional Yolk-Shell nanoparticles : a potential MRI contrast and anticancer agent[END_REF] Material In this section, we will first present the basis of NIR imaging and in particular the relevancy (i) of the NIR wavelength window for a high signal to background ratio (thanks to the high transmissivity of the organic tissue in this range of wavelengths) and (ii) of the QDs compared to other fluorescent probes. Then, we will focus on the existing synthetic routes with an emphasis on the development of non-toxic semiconductor nanocrystals (NCs) as alternative to Cd-, Pb-and Hg-based QDs. These approaches will be examined in the context of preparing NCs well-suited for in vivo imaging i.e. (i) small size to facilitate circulation and clearance and, (ii) narrow-size distribution and brightness to provide efficient detection at QDs concentration as low as possible.

III.1 Basics of NIR luminescence imaging

Context

Among the various modalities for bioimaging, fluorescence imaging is of special interest because of its low cost, high sensitivity, high spatial resolution and ease to implement (just with a low light camera). In the case of real time in vivo detection, the fundamental barriers to fluorescence imaging of a tissue are auto-fluorescence, high light scattering and absorption of the different tissue and blood components: water, haemoglobin, melanin, proteins…(Figure 5). [START_REF] Pansare | Review of Long-Wavelength Optical and NIR Imaging Materials: Contrast Agents, Fluorophores, and Multifunctional Nano Carriers[END_REF] Figure 5: Absorbance of various tissue and blood components from 200 nm to 10 µm.

Reprinted with permission from [START_REF] Pansare | Review of Long-Wavelength Optical and NIR Imaging Materials: Contrast Agents, Fluorophores, and Multifunctional Nano Carriers[END_REF] Copyright 2012. American Chemical Society.

These endogenous absorbers possess high absorption characteristics between 200-650 nm and thus, prevent light to penetrate deep into the tissues in the visible range. Moreover, the tissue auto-fluorescence also limits the signal-to-background ratio and hampers the detection of the fluorescent imaging agent. These intrinsic limitations have stimulated, in the last few years, the development of fluorescent probes with absorption and emission maxima in the 650-1450 nm range where tissues have minimal absorbance and fluorescence. . [START_REF] Pansare | Review of Long-Wavelength Optical and NIR Imaging Materials: Contrast Agents, Fluorophores, and Multifunctional Nano Carriers[END_REF][START_REF] Weissleder | A clearer vision for in vivo imaging[END_REF][START_REF] Frangioni | In vivo near-infrared fluorescence imaging[END_REF] As a general guideline, ideal fluorescent probes should fulfil also the following requirements [START_REF] Resch-Genger | Quantum dots versus organic dyes as fluorescent labels[END_REF] :

-Stability in biological media.

-Long fluorescence lifetimes for an efficient temporal discrimination from scattered excitation light.

-High brightness (product of high quantum yield, i.e. high number of emitted photons per number of absorbed photons, and high extinction coefficient).

-Narrow, symmetric emission bands and large Stokes shifts to easily separate the excitation and emission.

-No toxicity or interference with cell physiology.

The organic fluorescent dyes (cyanines, pyrroles-or porphyrins-based cycles, squaraines and borondipyrromethene classes) [START_REF] Pansare | Review of Long-Wavelength Optical and NIR Imaging Materials: Contrast Agents, Fluorophores, and Multifunctional Nano Carriers[END_REF] which were historically first used in NIR biodetection, 70 are far away to be ideal probes. In the far-red/near-infrared (NIR) wavelengths range, they suffer from rather low quantum yield, photobleaching (making them unsuitable for extended period of observation) and broad emission spectra which create overlapping detection ranges (inadequate for simultaneous multicolor applications). [START_REF] Pansare | Review of Long-Wavelength Optical and NIR Imaging Materials: Contrast Agents, Fluorophores, and Multifunctional Nano Carriers[END_REF][START_REF] Aswathy | Near-infrared quantum dots for deep tissue imaging[END_REF] Even if remarkable progresses have been made to improve the performances of dye-doped silica NPs and to develop new probes such as up-converting NPs [START_REF] Shan | The Hidden Effects of Particle Shape and Criteria for Evaluating the Upconversion Luminescence of the Lanthanide Doped Nanophosphors[END_REF][START_REF] Chatterjee | Small Upconverting Fluorescent Nanoparticles for Biomedical Applications[END_REF] absorption spectra, large two-photon action cross-section, and high photostability. [START_REF] Resch-Genger | Quantum dots versus organic dyes as fluorescent labels[END_REF] However, QDs suffer from the drawback of blinking (intermittence in light emission), which is problematic in case of single molecule tracking [START_REF] Baba | Single-Molecule Tracking in Living Cells Using Single Quantum Dot Applications[END_REF], instability of QY in different media and possible emission variability do to slight size modification between chemical batches.

QDs specificities

Owing to their nanoscale dimension, the intrinsic physical characteristics of the material are transformed by quantum effect below a certain size limit (Bohr radius) which ranges from ~2 nm to ~50 nm according to the material. [START_REF] Alivisatos | Perspectives on the Physical Chemistry of Semiconductor Nanocrystals[END_REF] At these sizes, nanocrystals lie in between the atomic and molecular limit (discrete density of electronic levels) and the extended crystalline limit (continuous bands i.e. the valence band and the conduction band) of bulk semiconductor.

This leads to size-dependent optical properties (Figure 6), [START_REF] De Mello Donega | Synthesis and properties of colloidal heteronanocrystals[END_REF] the maximum emission wavelength attainable being that of the bulk material.

Figure 6: Electronic energy states of a semiconductor in the transition from discrete molecules to nanosized crystals and bulk crystals. Blue shading denotes ground state electron occupation. Adapted with permission from [START_REF] Smith | Semiconductor Nanocrystals: Structure, Properties, and Band Gap Engineering Acc[END_REF] Copyright 2012. American Chemical Society.

When NCs is excited by quanta of energy, an electron is promoted from the valence band into the conduction band, leaving a hole in the valence band (electron-hole pair, i. e. exciton generation). The exciton recombination results in light emission at a wavelength longer than the absorbed light (Stokes shift). Several factors can be used to vary band gap and thus, to control absorption and luminescence wavelengths of the NCs. Classically, band gap engineering can be achieved through the variation of (i) the particle size, or (ii) of the composition. Several alternatives exist for modifying the band gap: (iii) doping the semiconductor host NCs with the incorporation of small amount of impurities, and (iv) modifying the internal structure (homogeneous vs. graded), for example in ternary system QDs like CdSe 1-x Te x . [START_REF] Bailey | Alloyed semiconductor quantum dots: tuning the optical properties without changing the particle size[END_REF] Thanks to these strategies, there are now a large variety of QDs that luminesce in the NIR region as illustrated in the figure 7. The references used for the figure are the following: II-VI, [START_REF] Bailey | Alloyed semiconductor quantum dots: tuning the optical properties without changing the particle size[END_REF][START_REF] Gaponik | Aqueous Synthesis of Semiconductor Nanocrystals in Semiconductor Nanocrystals Quantum Dots[END_REF]81,[START_REF] Pons | Synthesis of Near-Infrared-Emitting, Water-Soluble CdTeSe/CdZnS Core/Shell Quantum Dots[END_REF][START_REF] Harrison | Wet chemical synthesis and spectroscopic study of CdHgTe nanocrystals with strong near-infrared luminescence[END_REF][START_REF] Kovalenko | Colloidal HgTe Nanocrystals with Widely Tunable Narrow Band Gap Energies: From Telecommunications to Molecular Vibrations[END_REF] IV-VI, [START_REF] Cademartiri | Size-Dependent Extinction Coefficients of PbS Quantum Dots[END_REF][START_REF] Hines | Colloidal PbS Nanocrystals with Size-Tunable Near-Infrared Emission: Observation of Post-Synthesis Self-Narrowing of the Particle Size Distribution[END_REF][START_REF] Akhtar | Controlled Synthesis of Tuned Bandgap Nanodimensional Alloys of PbS x Se 1-x[END_REF][START_REF] Moreels | Composition and Size-Dependent Extinction Coefficient of Colloidal PbSe Quantum Dots[END_REF][START_REF] Murphy | PbTe Colloidal Nanocrystals: Synthesis, Characterization, and Multiple Exciton Generation[END_REF] III-V, [START_REF] Xie | Colloidal InP Nanocrystals as Efficient Emitters Covering Blue to Near-Infrared[END_REF][START_REF] Xie | Synthesis of Cu-Doped InP Nanocrystals (d-dots) with ZnSe Diffusion Barrier as Efficient and Color-Tunable NIR Emitters[END_REF][START_REF] Kim | Engineering InAs x P 1-x /InP/ZnSe III-V Alloyed Core/Shell Quantum Dots for the Near-Infrared[END_REF][START_REF] Xie | Synthetic Scheme for High-Quality InAs Nanocrystals Based on Self-Focusing and One-Pot Synthesis of InAs-Based Core-Shell Nanocrystals[END_REF]] II 3 -V2, [START_REF] Xie | Synthesis of Monodisperse, Highly Emissive, and Size-Tunable Cd 3 P 2 Nanocrystals[END_REF][START_REF] Harris | Synthesis of Cadmium Arsenide Quantum Dots Luminescent in the Infrared[END_REF] I-II-VI2, [START_REF] Xie | Formation of High-Quality I-III-VI Semiconductor Nanocrystals by Tuning Relative Reactivity of Cationic Precursors[END_REF][START_REF] Cassette | Synthesis and Characterization of Near-Infrared Cu-In-Se/ZnS Core/Shell Quantum Dots for In vivo Imaging[END_REF] IV [START_REF] Ruddy | Size and Bandgap Control in the Solution-Phase Synthesis of Near-Infrared-Emitting Germanium Nanocrystals[END_REF][START_REF] Lee | Colloidal Synthesis of Infrared-Emitting Germanium Nanocrystals[END_REF] and I2-VI [100,101].

Finally, one can find a last strategy for designing NIR-emitting QDs that is based on core/shell C/S architecture: the core and shell are rationally chosen in order to favor the relaxation of a conduction-band electron of the core into the valence band of the shell (type-II QDs) (Figure 9c).

[102] The staggered band alignment leads to a smaller effective band gap than each one of the constituting core and shell materials. This aspect will be described in more details in the "Coating the active core" section devoted to heteronanocrystal, i.e. NCs incorporating two or more materials organized in C/S or core/multishells architecture.

III. 2. Luminescent semiconductor nanocrystals: chemical synthesis of NIR

emitting core NCs.

The literature reports a large variety of Cd, Pb or Hg based QDs for which the synthetic routes can be generally classified in two families, according the synthetic medium (aqueous or not). Different protocols have been described in water to produce II-VI semiconductors such as CdTe, CdSe x Te 1-x , HgTe, Cd x Hg 1-x Te, or Cd x Hg 1-x Se QDs.

[103] The major advantages of this aqueous medium approach are (i) the environmentally friendly medium, (ii) the ease to scale up to gram scale amounts for commercial purpose and (iii) the aqueous compatibility for applications, in particular, biomedical imaging.

[104] However, the size distribution is often broad and post-preparative procedures (size-selective precipitation) are required. [START_REF] Gaponik | Aqueous Synthesis of Semiconductor Nanocrystals in Semiconductor Nanocrystals Quantum Dots[END_REF] In this context, the development of the alternative hot injection method, i. While the use of precisely-controlled reaction conditions (air-and water-free atmosphere) can be seen as a major drawback when aiming at simple and straightforward procedures, these requirements offer, on the other side, the opportunity to introduce novel precursors yielding to unexplored materials for NCs such as the tin and germanium chalcogenides. ii. Synthesis of III-V semiconductors NCs (InP, InAs).

Following the same tendency toward "greener" material, III-V semiconductors are generally viewed as a highly relevant alternative. This is in particular the case for InP NCs which has been rapidly identified as one of the most promising alternatives to Cd-and Pb-based QDs and has focused the majority of the research efforts devoted to III-V QDs. InP NCs were first prepared in 1994 [116] following the, at the time recently published, hot-injection procedure developed for CdE (E = S, Se, Te) QDs with indium oxalate and tris(trimethylsilyl)phosphine (P(SiMe 3 ) 3 ). Longer reaction times (3-7 days) were required to yield good cristallinity. The progresses towards an easy, reliable and controlled synthesis (i.e. in non-coordinating solvent) followed those to their II-VI analogues,[117] but remain one step behind in particular for the size control. The preparation QDs size larger than 5 nm is still a challenging question. This issue is of central importance because, absorption wavelengths higher to 650 nm are at the upper limit of the current attainable range with InP. [START_REF] Xie | Colloidal InP Nanocrystals as Efficient Emitters Covering Blue to Near-Infrared[END_REF] It has recently been shown that the formation of a mixed oxide shell InPO x at the surface of the NCs is probably the reason of this growth inhibition. This is the consequence of the oxophilic character of phosphorus and of a side-reaction of the carboxylate ligand occurring at the temperature (230°C-300°C) required for the formation of NCs, which generates oxidative condition in the reaction medium.

[118]

However, the doping strategy proved to be successful and allow reaching emission wavelength up to 1100 nm. [START_REF] Xie | Synthesis of Cu-Doped InP Nanocrystals (d-dots) with ZnSe Diffusion Barrier as Efficient and Color-Tunable NIR Emitters[END_REF] InAs NCs were also prepared following the hot-injection method by typically the reaction of As(SiMe 3 )

IV. Surface modification and probe development

In view of their applications for biological imaging, NPs cannot be use directly after their synthesis for two major reasons. First, because nano-objects have high surface to volume ratios, a large fraction of the constituent atoms are located on the surface. These atoms are incompletely bonded within the crystal lattice, thus disrupting the crystalline periodicity and leaving one or more "dangling orbital" on each atom pointed outward from the crystal. While partially stabilized through dative ligand-metal bonds, the organic passivation is generally insufficient to provide inertness to the biological medium and/or to air. These surface atoms, indeed, remain highly reactive and are usually prone to oxidation. A general strategy to improve NPs' surface passivation is the overgrowth of a protecting shell around the core, affording chemical stability and preservation of the physical properties. A second requirement aiming at exploiting the magnetic or luminescent properties for biodetection is the solubility of the NPs in physiological media. As discussed in the previous sections, the NPs of best quality are generally produced in non polar solutions using aliphatic coordinating ligand making them insoluble in water. In this context, the phase transfer is an essential but nontrivial step before envisioning their use for biodetection. Finally, the surface of these watersoluble C/S NPs often needs to be engineered for in-vivo applications in order to increase the circulation time in the blood stream and enhance their targeting efficiency. The final object is then composed, as depicted in figure 8, of an inorganic core with optimized physical properties, surrounded by an inorganic shell and an organic corona composed of hydrophilic ligands and targeting molecules. . Thus, multi-steps physical approach (lithographic process, multiple metal evaporations), though time consuming, have been so far preferred for Co@Au NPs tested for MRI [START_REF] Bouchard | Picomolar sensitivity MRI and photoacoustic imaging of cobalt nanoparticles[END_REF] Oxide shells are alternative candidates which benefits from i) fairly low toxicity levels

[136] and ii) simple chemical strategies. The simplest choice relies on the oxide shell which naturally grows at the surface of the metallic core exposed in air. For instance, the native CoO shell is an efficient passivating layer for Co core. In the case of Fe, the stability of Fe@Fe 3 O 4 requires a crystalline oxide shell [129]. While such shell is naturally obtained on single crystalline Fe core [START_REF] Lacroix | Stable singlecrystalline body centered cubic Fe nanoparticles[END_REF] a controlled oxidation process at high temperature is required for amorphous Fe core [129]. Though CoO and crystalline Fe 3 O 4 confer air-stability, these shells are stable in aqueous media only in a selected pH and ionic strength range. Therefore, SiO 2 coating, due to its remarkable stability in water, has been extensively studied [137]. Silica coating is often grown through water-in-oil microemulsion which may induce an oxidation of the metallic core, thus alternative approaches based on non-alcoholic solvants should be preferred [138,139]. Additionally, silica shell grown in liquid phase, is generally not fully condensed (incomplete hydrolysis and condensation steps). Thus, post-treatments (annealing as example) are required to make it denser and to prevent a possible permeation to oxygen or any leaching of metallic ions from the core. To the best of our knowledge, such M@SiO 2 NPs (M= metal) with a well-condensed shell have never been tested so far neither in vitro nor in vivo.

Finally, graphitic shell can also be grown to stabilize metallic core either through the calcination of the surrounding ligands [START_REF] Desvaux | Multimillimetre-large superlattices of air-stable iron-cobalt nanoparticles[END_REF] or through chemical vapor deposition (CVD) [START_REF] Seo | FeCo/graphitic-shell nanocrystals as advanced magnetic-resonance-imaging and near-infrared agents[END_REF].

Such shell has the advantages of being thin, functionalizable and up-to-now, no negative health problems were detected [START_REF] Seo | FeCo/graphitic-shell nanocrystals as advanced magnetic-resonance-imaging and near-infrared agents[END_REF]. However, coating of highly reactive Fe NPs should be tested to conclude on the efficiency of such C shell towards oxidation.

b) Quantum dots

In the case of QDs, the role of the shell goes well beyond the sole function of protecting against oxidation and photo-oxidation. The dangling orbitals of the under-coordinated atoms located at the surface may form energy states ("surface energy state") which quench the luminescence through non-radiative decay paths (Figure 9a). [START_REF] Smith | Semiconductor Nanocrystals: Structure, Properties, and Band Gap Engineering Acc[END_REF] When coating, the dangling bonds are passivated with atoms of the shell, resulting in the dramatic enhancement of the photoluminescence efficiency. As an example, the QY of naked InP NCs is generally inferior to 0.1% but after being coated with ZnS, the QY of the resulting InP/ZnS C/S QDs increases up to 22%. [140] In the majority of cases, the materials chosen for shell are semiconductors which have a wider band gap than those of core (C/S system called type-I structure) in order to provide electronic insulation thanks to the confinement of both electrons and holes in the core (Figure 9b). A representative (but not exhaustive) list of commonly encountered compositions for NIR emitting C/S NCs is CdTe/MS (M=Zn, Cd), HgTe/CdS, PbSe/PbS, PbSe/CdSe, InP/ZnE (E= S, Se), InAs/InP, InAs/GaAs, InAs/CdSe, Cd 3 P 2 /ZnS, CuInE/ZnS (E= S, Se). [START_REF] Xie | Formation of High-Quality I-III-VI Semiconductor Nanocrystals by Tuning Relative Reactivity of Cationic Precursors[END_REF]102,112] For bio-applications, the shell is generally composed of non toxic elements (e.g. ZnS, prepared with zinc stearate and dodecanethiol) to minimize potential toxic effect by preventing the leaching of element from the core.

[102] A general requirement for obtaining highly luminescent C/S QDs is the epitaxial growth of the shell and thus, the use of a material which crystallizes in the same structure than that of the core and has small lattice mismatch with it.

[141] The shelling of the QDs is achieved through the slow addition (in order to avoid side-nucleation and formation of separate NCs composed of the shell materials)

of the shell precursors into a solution of the purified core. An example of this kind of C/S architecture is InAs x P 1-x /InP/ZnSe alloyed QDs for which ZnSe was chosen of its better lattice match to InP than ZnS. [START_REF] Kim | Engineering InAs x P 1-x /InP/ZnSe III-V Alloyed Core/Shell Quantum Dots for the Near-Infrared[END_REF] Figure 9. Core a) Type-I, b) and type-II core-shell, c) band-edge alignments at the surface and the heterointerface between two semiconductors. In the type-I structure, both the electron and the hole localize within the material with a narrower energy gap, which is semiconductor 1 (sem1) in the present case. As a result, the wavelength emission, λ 1 , is determined by E g1 .

The energy gradient existing in the type-II structure tends to spatially separate the electron and the hole on different sides of the heterointerface. In this case, the wavelength emission λ 2 is determined by the energy difference between the conduction band edge of sem1 and the valence band edge of semiconductor 2 (sem2), and hence, it is lower than the band gap of either semiconductor. Adapted with permission from [ 142 ] Copyright 2012. American Chemical Society.

Interestingly, by choosing appropriately the shell material, it is possible to tune the emission at wavelengths that cannot be achieved with any of the two materials (those of core and shell) alone. In this type-II system, both the valence and the conduction bands of the shell are lower (or higher) than in the core. As a consequence, this band alignment leads to smaller effective bandgap than each one of the core and the shell material (Figure 9c). This approach is particularly relevant for attaining near-infrared window: for instance, the emission wavelength of the CdTe/CdSe and CdSe/ZnTe C/S heterostructures could be tuned in the NIR range while these emission wavelengths would not be reached by increasing the size of the respective Last, the blinking of QDs which is highly detrimental to their use for single molecule tracking [START_REF] Baba | Single-Molecule Tracking in Living Cells Using Single Quantum Dot Applications[END_REF] can be suppressed by the coating with thick shells (i.e. 20 monolayers) yielding to a final diameter of ~15 nm.

[144] The major drawback is the large size that may be inappropriate for the observation of molecular phenomenon, [START_REF] Baba | Single-Molecule Tracking in Living Cells Using Single Quantum Dot Applications[END_REF] but this problem have been shown to be possibly circumvented when a composition-graded interface exists between the core and the shell in the more compact (8 nm) CdSe/ZnSe QDs.

[145]

IV.2. Phase transfer and surface modification.

a. Phase transfer -water stability -stealth Phase transfer became an important issue since optimized functional nanoparticles have been prepared in organic solvent, different strategies have been already reviewed [146,147] and can be sorted, in a first approximation, between two generic approaches (Figure 10):

-ligand exchange : hydrophobic surfactants are replaced by a bifunctional ligand presenting at one end, a function holding a stronger affinity with the NPs surface than the initial ligand and, at the other side, a hydrophilic ending. To enhance the binding affinity and favour a complete replacement of the hydrophobic surfactants, polydendate ligands, such as dimercaptosuccinic acid (DMSA), are often used [START_REF] Huh | Artificially engineered magnetic nanoparticles for ultra-sensitive molecular imaging[END_REF]. This ligand exchange approach is particularly useful to stabilize water-soluble nanoparticles with small hydrodynamic size (<20nm), but may lead to particle aggregation and loss of optical properties for QDs The choice of the functionalization strategy results from a delicate balance between the surface state chemistry of the NPs and the final hydrodynamic diameter reached.

Hydrodynamic size influences the relaxativity constant and drives the interactions with tissues and biological media (through size dependent diffusion). While ultra-small particles (ca. 5nm) are quickly excreted by the kidney, intermediate NPs (15-100 nm) exhibit longer circulation time [152],larger NPs (> 100 nm) being more susceptible to opsonisation (uptake by the immune defence system). Thus, the functionalization strategy must be carefully chosen in order to reach the optimized window of hydrodynamic size (15-100nm).

In addition to the hydrodynamic size effect, the pharmacokinetics and biodistribution of nanoparticles is driven by surface coating. Lifetime in blood circulation strongly depends on the interaction of the NPs with plasma proteins (opsonins). Accumulations of opsonins are recognized by reticuloendothelial system (RES) and phagocyted by macrophages Grafting of PEG on the surface of NPs may inhibit the protein interaction and prolong the blood circulation time.

[153] This effect strongly depends on the conformation of the PEG chains at the NPs surface, which evolves from mushroom to brush configurations for longer PEG chain Small molecules, peptides, proteins, aptamers and antibodies have demonstrated high affinity with receptors overexpressed in malignant cells as previously reviewed. [START_REF] Cho | Inorganic nanoparticle-based contrast agents for moleuclar imaging[END_REF][START_REF] Yang | Emerging inorganic nanomaterials for pancreatic cancer diagnosis and treatment[END_REF]153]. A key issue during the grafting of such moieties onto the NP surface is to maintain their affinity for receptors. Their density, accessibility and conformation should be preserved, thus, spacers are often added to avoid shielding and denaturing of the ligand.

V. Applications

In this part, we aim to illustrate the recent progress in MRI and NIR in vivo real time imaging due to the use of new generation of magnetic nanoparticles and QDs. A last part will aim at presenting the recent very first tries of combination of both properties in multimodal single nano-objects and the promises of this strategy.

V.1 MRI in vivo

In this part, we aim to illustrate the recent progress in in vivo MRI due to the use of new shown that Fe/FeOx core/shell NPs improve by a factor 2 the contrast in T2-weighted MR images of mice nodes compared to pure FeOx NPs. Interestingly, they allow for a much better in vivo detection of small tumors (1-3 mm) at 1.5 T. [START_REF] Cheong | Simple synthesis and functionalization of iron nanoparticles for magnetic resonance imaging[END_REF] In vivo probing of small-sized cancers (~50 mg) with manganese ferrites NPs coated with DMSA and conjugated with the cancer-targeting antibody Herceptin was successful too as reported by the Cheon's group. [START_REF] Huh | Artificially engineered magnetic nanoparticles for ultra-sensitive molecular imaging[END_REF]. On the contrary, the analogue pure iron oxide nanoparticles did not allow such performances. The authors attribute this promising result to the higher saturation magnetization of the manganese ferrites nanoparticles. Developed by Chen et al., the 12 nm-FePt nanoparticles conjugated to the anti-Her2 monoclonal antibody showed significant contrast enhancement in both MRI and computated tomography (CT), thus taking advantage of their magnetic properties and the high X-ray absorption of platinum.

[159] Indeed, 24h

after injection (28 mM Fe concentration, 100 µL) into mice bearing transplanted MBT2 tumor, the MR images showed 51% intensity reduction on the tumor lesion while CT image analysis revealed 138% contrast enhancement. In addition, the biodistribution of the nonfonctionalized FePt nanoparticles evaluated on mice suggest that they could be cleared from the body after about 1 week.

The FeCo@graphitic carbon (GC) nanocrystals prepared by Dai et al. showed unusually higher r1 and r2 values than conventional Gd and iron-oxide-based contrast agents [START_REF] Seo | FeCo/graphitic-shell nanocrystals as advanced magnetic-resonance-imaging and near-infrared agents[END_REF]. As an example, they allowed for positive contrast enhancement on T1-weighted MR images of the blood pool in the rabbit (see Figure 11). 12). Interestingly, this degree of sensitivity is approaching the one of radioactive labels. PAT detection was also conclusive as observe for a rat tail local injection of 100 pM of nanowontons. properties nor their relaxativity. In order to favour metallic materials which exhibit higher magnetization, a solution consists in incorporating preformed magnetic NPs and QDs into an isolating matrix (such as silica).

V.2 Luminescence

[ 176 ] However, the resulting object exhibits a high hydrodynamic volume, which may be a drawback for further in-vivo applications and prevents the diffusion of water proton at the vicinity of the magnetic NPs, resulting in poor relaxativity.

[177] Deka et al. have reported a promising approach based on the intercalation of a semiconductor with larger band gap between the metallic part and the QD, which may result in decoupling QD and metal electronic states.

[178] CdSe@CdS decorated with Co tips exhibited preserved magnetic properties (M S =148 emu/g Co ) but partially quenched fluorescence (QY = 3%). Optimization of the spacer nature and thickness could be pursued to retain both physical properties unaltered.

Conclusion :

In Cd-free InP/ZnS QDs. The next step towards the optimization of contrast agents relies on the integration, within a single object, of MRI and NIR imaging potentialities. Such multimodal NPs, though extremely promising, requires the strict decoupling of semiconducting and metallic electronic states. The introduction of a large gap semiconductor spacer could be the most promising approach which could yield to unaltered magnetic and optic properties.

Figure 2 .

 2 Figure 2. Schematic view of water proton spins in a) a static magnetic field B 0 and b) upon RF-excitation Dashed arrow represents M Z component, solid circle represents M X,Y component. Evolution as a function of time of d)M Z and e) M X,Y with respectively T 1 and T2 as time constant derived from the initial slope (dashed lines).

Figure 3 .

 3 Figure 3. Schematic view of a magnetic nanoparticle surrounded by water protons. Red arrow indicate the magnetic field induced.

Figure 7 :

 7 Figure 7: Compositions, sizes and wavelengths ranges of reported NIR-emitting QDs prepared via solution-based methodologies. Emission wavelengths reported for constant size NCs containing different proportions of elements are represented with broken lines rectangle. The references used for the figure are the following: II-VI,[START_REF] Bailey | Alloyed semiconductor quantum dots: tuning the optical properties without changing the particle size[END_REF][START_REF] Gaponik | Aqueous Synthesis of Semiconductor Nanocrystals in Semiconductor Nanocrystals Quantum Dots[END_REF] 81,[START_REF] Pons | Synthesis of Near-Infrared-Emitting, Water-Soluble CdTeSe/CdZnS Core/Shell Quantum Dots[END_REF][START_REF] Harrison | Wet chemical synthesis and spectroscopic study of CdHgTe nanocrystals with strong near-infrared luminescence[END_REF][START_REF] Kovalenko | Colloidal HgTe Nanocrystals with Widely Tunable Narrow Band Gap Energies: From Telecommunications to Molecular Vibrations[END_REF] IV-VI,[START_REF] Cademartiri | Size-Dependent Extinction Coefficients of PbS Quantum Dots[END_REF][START_REF] Hines | Colloidal PbS Nanocrystals with Size-Tunable Near-Infrared Emission: Observation of Post-Synthesis Self-Narrowing of the Particle Size Distribution[END_REF][START_REF] Akhtar | Controlled Synthesis of Tuned Bandgap Nanodimensional Alloys of PbS x Se 1-x[END_REF][START_REF] Moreels | Composition and Size-Dependent Extinction Coefficient of Colloidal PbSe Quantum Dots[END_REF][START_REF] Murphy | PbTe Colloidal Nanocrystals: Synthesis, Characterization, and Multiple Exciton Generation[END_REF] III-V,[START_REF] Xie | Colloidal InP Nanocrystals as Efficient Emitters Covering Blue to Near-Infrared[END_REF][START_REF] Xie | Synthesis of Cu-Doped InP Nanocrystals (d-dots) with ZnSe Diffusion Barrier as Efficient and Color-Tunable NIR Emitters[END_REF][START_REF] Kim | Engineering InAs x P 1-x /InP/ZnSe III-V Alloyed Core/Shell Quantum Dots for the Near-Infrared[END_REF][START_REF] Xie | Synthetic Scheme for High-Quality InAs Nanocrystals Based on Self-Focusing and One-Pot Synthesis of InAs-Based Core-Shell Nanocrystals[END_REF]] II 3 -V2,[START_REF] Xie | Synthesis of Monodisperse, Highly Emissive, and Size-Tunable Cd 3 P 2 Nanocrystals[END_REF][START_REF] Harris | Synthesis of Cadmium Arsenide Quantum Dots Luminescent in the Infrared[END_REF] I-II-VI2,[START_REF] Xie | Formation of High-Quality I-III-VI Semiconductor Nanocrystals by Tuning Relative Reactivity of Cationic Precursors[END_REF][START_REF] Cassette | Synthesis and Characterization of Near-Infrared Cu-In-Se/ZnS Core/Shell Quantum Dots for In vivo Imaging[END_REF] IV[START_REF] Ruddy | Size and Bandgap Control in the Solution-Phase Synthesis of Near-Infrared-Emitting Germanium Nanocrystals[END_REF][START_REF] Lee | Colloidal Synthesis of Infrared-Emitting Germanium Nanocrystals[END_REF] and I2-VI[100, 101].

  e. the synthesis of NCs in high-temperature boiling organic solvents is considered as one of the main milestones in the chemistry of QDs. The temporal separation of the nucleation and the growth of the seeds gave access to high quality NCs with narrow size distribution (5-10% standard deviation) without laborious size selective precipitation procedure. Since the early works (preparation by Murray et al. of CdE (E = S, Se, Te),[105] synthetic improvements have allowed an ongoing trend toward simpler and safer procedures (replacement of the hazardous [106] or expensive chemicals,[107] decrease of the reaction temperature until ~100 °C [108]).Moreover, the widespread success of the hot-injection strategy is also largely due to its versatility in particular, in terms of chemical variety. The extension of the list of semiconductor materials to high quality (in terms of monodispersity and optical emission) IV-VI QDs such as PbE (E= S,[START_REF] Hines | Colloidal PbS Nanocrystals with Size-Tunable Near-Infrared Emission: Observation of Post-Synthesis Self-Narrowing of the Particle Size Distribution[END_REF] Se, [ 109 ] Te [ 110 ]), is one of the valuable consequences.[ 111] Finally, emerging materials such as II 3 -V 2 are also worth citing: for instance, a room temperature procedure has recently be developed to yield Cd 3 P 2 QDs which emit in the NIR region[112] and can be envisioned for biodetection. It should also be noted that in case of mercury-based NCs, the aqueous strategy remains the best-suited and almost exclusive approach.[103, 111] In the context of in vivo applications, the issue of metabolic clearance is still an open and unresolved question. To avoid any dilemma, one strategy is to extend the NCs family toward more environmentally friendly elements than Cd, Pb or Hg.[113] We have chosen to detail this attractive perspective in the following paragraphs.i. Synthesis of Pb-free IV-VI semiconductors NCs (GeE, SnE, E= S, Se, Te).

  [ 114 ] The preparation of SnTe NCs [ 115 ] using the sophisticated tin complex bis[bis(trimethylsilyl)amino]tin(II) (Sn[N(SiMe 3 ) 2 ] 2 ) and trioctylphosphine telluride (TOPTe) was the starting shot toward materials involving these lighter elements of the Pb group. Today, a large variety of compositions (GeS, GeSe, GeTe, Ge x Sn 1-x Se, SnS x Se 1-x …) and morphology (sphere, sheet, needle) with tunable band gap in the NIR region is accessible.[114] Although the emission properties has not yet been explored, tin and germanium monochalcogenide represent very promising material which would deserve to be tested in the context of biodetection.

Figure 8 .IV. 1 .

 81 Figure 8. Schematic view of a surface engineered active core (gray) coated with an inorganic shell (blue), hydrophilic surfactants (light gray) and targeting agents (red).

  CdTe or CdSe cores.[143] In general, type II C/S QDs have low QY and low photochemical stabilities because one charge (either the electron or the hole) localized in the shell is in direct contact with the surrounding medium and, thus similar reactions than those of naked QDs may occur.[134] These two properties can be improved by coating with another semiconductor material to yield a core multishell structure.[102]

  [147]. This problem is commonly encountered for C/S QDs such as CdSe/ZnS,[148] InP/ZnS [149] or the other NIR-emitting material CuInS 2 /ZnS.[150] Recently, Reiss et al. have given insight on the precise mechanism, attributing the quenching to hole transfer from the QDs to the capping ligand (cysteine) resulting in the formation of the cysteine dimer (cystine).[150] -copolymer addition : amphiphilic surfactants are added, their hydrophobic tails form weak interactions with the existing hydrophobic coating while their hydrophilic groups are exposed, ensuring the water-solubility. Variety of lipophilic polyethylene glycol (PEG)-based polymers have been used [147] Such copolymer strategy leads to a drastic increase of the hydrodynamic size of the NPs (>20nm) but ensures a fairly long blood circulation due to PEG moities [151].

Figure 10 .

 10 Figure 10. Schematic view of the three generic strategies for water transfer of hydrophobic NPs : through ligand exchange or copolymer addition.

(≥ 2000

 2000 Da) and higher surface density. [153] While brush configurations generate greater protein repulsion, it may also lower the nanoparticle targeting efficiency due to the sterically shielding of the specific agents. [154] Therefore, targeting agents should be conjugated to PEG-spacer of similar length to stand at the outmost exterior of the NPs, lying above the organic corona. [153] b. Cancer cell targeting Numerous reports have shown that most NPs accumulate in tumors due to enhanced permeation and retention (EPR) effect, which results from relatively large and permeable blood vessels along with poor lymphatic drainage of tumor cells. [153] For instance, iron oxide NPs were successfully used to diagnose cancer without any targeting agents [155]. Suchcancer cell uptake strategy is referred to as passive targeting and let consider a possibility of universal labeling. Charged NPs have been tested in the seeking of universal labeling but controversial results have been found. While anionic NPs (citrate) have been reported as exhibiting a better cell-uptake than cationic or uncharged NPs,[156] another study shows that cationic (aminodextran) NPs were optimized. [157] Though contradictory, these results might be explained by the tendency of charged NPs to be destabilized under harsh pH and ionic strength environment, as encountered in biological media.In order to enhance the selective internalization of NPs, active targeting strategies were developed. Driven at the vicinity of tumor cells by EPR effect, NP grafted with adequate moieties would be internalized faster through receptor-mediated endocytosis. Such tumor surrounding clearance generates a diffusion gradient which can favor the further NP flow, and thus, the accumulation of NP within the tumor region.[153] One of the main challenges of active targeting is the design of adequate targeting moieties. Indeed, tumor cells exhibit receptors fairly similar to the surrounding healthy cells, the difference being their relative abundance. Therefore, targeting agent must specifically bind to overexpressed receptors.

Figure 11 .

 11 Figure 11. T1-weighted MR images of a rabbit a) before and b) 30 min after initial Injection of a solution of 4nm FeCo/GC nanocrystals (metal dose 9.6 µmol.kg-1 for the 5kg rabbit). The blood pool in the aorta is significantly brightened (positive contrast) in the MRI after injection. We also see signal increase in the kidney medulla and cortex due to the high blood volume within the kidney. We see little signal enhancement in the muscle. Reprinted with permission from Macmillan Publishers Ltd : Nature Materials[START_REF] Seo | FeCo/graphitic-shell nanocrystals as advanced magnetic-resonance-imaging and near-infrared agents[END_REF].Copyright 2006.

Figure 12 .

 12 Figure 12. Transverse (axial) MRI image in mouse leg muscle injected with Co nanowontons in PBS solution. The position of the blue arrows indicates the sites of injection for the nanowontons (upper right corner) and the PBS control (lower left corner). Two watercarrying test tubes are also visible in the scans for purposes of MRI slice alignment (red arrows). MRI parameters were: TE = 50 ms; TR = 1 s; field of view is 2.6 cm × 2.6 cm, and slice thickness is 0.5 mm.

  As a representative example of the potential of such a tool for realtime in vivo visualization, Reiss et al. monitored the fluorescence distribution of CuInS 2 /ZnS QDs (functionalized with dihydrolipoic acid yielding a hydrodynamic diameter of ~17 nm) with time (Figure13). [163] QDs were injected intravenously into the tail of nude mouse and after 15 min, they accumulate essentially in the liver, spleen and lungs (fluorescence in the stomach is attributed to the feed).

Figure 13 .

 13 Figure 13. a) Fluorescence images (excitation wavelength 633 nm) showing the temporal evolution of the biodistribution of the CuInS 2 /ZnS NCs injected intravenously into the tail of a healthy nude mouse (eq 6.5 × 1016 to 1.3 × 1017 copper atoms). The integration time is 200 ms and the contrast has been set between 1850 and 32400. b) Fluorescence images of the different parts of the mouse after dissection. Adapted with permission from [163] Copyright 2012. American Chemical Society.

Figure 15 .

 15 Figure 15. The dorsal images of SKOV3 tumor-bearing (arrows) mice injected with (A) InP/ZnS-Dendron-RGD2 (200 pmol) and (B) InP/ZnS-Dendron (200 pmol) at 0.5, 1, 4, 5, 5.5, 6, 8, 24, and 28h, respectively. The incidental high fluorescent signals in other body parts (arrowheads) might have originated from regular rodent food in stomach and feces in intestine. Reprinted with permission from [166] Copyright 2012. American Chemical Society.

  this review paper, we have presented the potentiality of a new generation of optimized contrast agents, based on metallic NPs and Hg, Cd, Pb, As free QDs, for respectively MRI and NIR imaging. Though extensive literatures can be found on well established iron oxide NPs or Cd-based quantum dots, only few reports outline the requirements that new probe generation should fulfil. Thanks to the description of the physics of the imaging techniques, optimized materials could be enlightened as long as the syntheses which yield to the corresponding NPs. Surface engineering strategies to ensure the biodistribution and the specific targeting of inorganic NPs were reviewed. The resulting NPs combines, through a complex architecture, the optimized inorganic core surrounded by a non-porous coating shell, to ensure the stability of the core, an organic corona to reach adequate biodistribution and targeting moities to enhance the specific cellular uptake. Few results demonstrate the in vivo potentiality of these new generations of probes. Drastic enhancement of relaxativity (up to 10 5 times) was observed for Co based NPs, while impressive fluorescent results were obtained for

Table 2 .

 2 Overview

of the chemical approaches for the synthesis of metallic NPs. OA: oleic acid. OY: oleylamine. HDAHCl: hexadecylamonium chloride. NaOA : sodium oleate. PA: palmitic acid. HDA: hexadecylamine. LA: lauric acid. DDA: dodecylamine. PMMA: polymethylmethacrylate. PEG: polyethyleneglycol. TOP: trioctylphosphine. TOPO: trioctylphosphine oxide. DOA: dioctylamine. SA: Stearic acid III. NIR detection principle and NIR luminescent semiconductor nanocrystals:

  or noble metal (gold and silver) nanoclusters,

	[Erreur ! Signet non défini., 74] the optical performances (especially QYs) are not yet
	competitive enough.
	Among the NIR fluorescent probes, [Erreur ! Signet non défini.] quantum dots (QDs) offer
	today the best optical properties and appear as a very powerful and essential tool in
	biodetection. Indeed, they exhibit large molar extinction coefficients, high QY (> 50%),
	narrow and symmetric photoluminescence (PL) emission bands, size-tunable emission and

  Over the last decade, significant progresses have been made concerning the chemistry of NCs of materials alternative to II-VI, IV-VI and III-V. So far, two main families have focused the majority of the research efforts: elemental group IV (Si, Ge) semiconductors and I-III-VI 2

	chalcopyrite types like CuInE 2 (E = S, Se) or AgInS 2 . [96] In the latter case, the synthetic
	strategy is essentially the same than the one developed in the hot injection method for II-VI,
	IV-VI and III-V materials, i.e. in coordinating (TOPO) [ 121 ] or non-coordinating
	(dioctylphtalate,[122] ODE [123]) solvents. Concerning group IV elements NCs, the synthesis
	is far less developed. Two main solution strategies exist and involve either strong reducing
	agents (zintl salts, LiAlH
	3 and indium chloride [119] or acetate.[117] In
	the latter case, the QDs size can be controlled to access a range of emission wavelength well-
	suited for biodetection purpose i.e. between 700 and 1400 nm, with diameters less than ∼6
	nm.[93]As example, InAs NPs of 3.2 nm of diameter emitting at 750 nm can be easily cleared
	from the body.[120]

iii. Others semiconductors (IV, I 2 -VI and I-III-VI 2 types) for NIR emitting NCs. 4 , K/Na alloy) and/or high-temperature procedures (usually supercritical thermolysis condition).

[START_REF] Ruddy | Size and Bandgap Control in the Solution-Phase Synthesis of Near-Infrared-Emitting Germanium Nanocrystals[END_REF]

An exception from this rule, is the approaches developed by Boyle's [124] and Klimov's

[START_REF] Lee | Colloidal Synthesis of Infrared-Emitting Germanium Nanocrystals[END_REF]

groups who took advantage of the reactivity of Ge(II) precursors using hot injection approach. Very recently, silver chalcogenide Ag2E

[101]

and in particular silver sulfide Ag 2 S [125] were identified as promising materials for NIRemitting QDs. For these NCs, both aqueous [100, 126, 127] and organic

[101, 125, 128]

solvents approaches were developed with similar results in terms of size distribution and optical quality, which open the way for in vivo studies.

[100,126]

  generation of magnetic nanoparticles. The main objective is to evaluate the potentialities of the latter to favour further developments in this field of application. Reviews on MRI using "classical" MNPs (SPIO, USPIO) can be referred to for comparison purpose; they generally describe in vivo MRI experiments dealing with cancer, cardiovascular disease or molecular imaging.[158] Here, we only report examples of MRI improvements due to new contrast agents. Moreover, we like to mention studies that directly compare MNPs whose magnetic materials were of different nature, but coating and functionalization were identical. This way, the other parameters that necessarily impact the MRI response (coating thickness, bio-distribution…) can be considered unchanged.As previously explained, the main reason to work on magnetic composition of contrast agents, is to enhance the contrast on MR images. In a recent study reported byCheong et al., it was

  Au nanowontons reported by Bouchard et al. were dual-modality MRI/photoacoustic tomography (PAT) contrast agent.[START_REF] Bouchard | Picomolar sensitivity MRI and photoacoustic imaging of cobalt nanoparticles[END_REF] Even when injected in mice muscle leg at concentration as low as 50 pM, a negative contrast was clearly detected on T 2 -weighted spin echo MR images (see Figure

	The Co@
	This was 30min after NPs injection using a metal dose of only 10% of what was typically
	used for existing Gd agents (metal dose ∼9.6 µmol kg-1 for the ∼5 kg rabbit). The authors
	claim that this represents an important achievement in MRI contrast-agent development; long-
	circulating positive-contrast enhancement at low metal dosages in vivo is indeed particularly
	interesting for angiographic MR images.

30 min after initial Injection of a solution of 4nm FeCo/GC nanocrystals (metal dose 9.6 µmol.kg-1 for the 5kg rabbit). The blood pool in the aorta is significantly brightened (positive contrast) in the MRI after injection. We also see signal increase in the kidney medulla and cortex due to the high blood volume within the kidney. We see little signal enhancement in the muscle. Reprinted with permission from Macmillan Publishers Ltd : Nature Materials

[START_REF] Seo | FeCo/graphitic-shell nanocrystals as advanced magnetic-resonance-imaging and near-infrared agents[END_REF]

.

Copyright 2006.

  Thanks to their remarkable features, NIR emitting QDs have become one of the mainstays of in vivo imaging modalities.[160] This success story started a decade ago with the real-time mapping of sentinel lymph nodes in mouse and pig, using type II C/S CdTe/CdSe QDs.[161] Since this significant achievement, progresses have been made in several main domains: biodistribution of QDs, tumors imaging, tracking of cells and vascular imaging (blood vessel and lymphatic circulatory system).[104, 160] Unfortunately, these results have been obtained using toxic elements such as Cd, Pb, Hg, or As. The toxicity concerns associated to this family of materials have fueled researches for their replacement with non-toxic elements. The relevancy of these materials (CuInE 2 /ZnS,[START_REF] Cassette | Synthesis and Characterization of Near-Infrared Cu-In-Se/ZnS Core/Shell Quantum Dots for In vivo Imaging[END_REF] 162, 163, 164, 165] InP/ZnS, [166] , Ag 2 E [100, 126] with E= S, Se) for in vivo NIR imaging have been proven in the very recent years in the context of biodistribution,[163] tumor[162, 166]and lymph imaging.[START_REF] Cassette | Synthesis and Characterization of Near-Infrared Cu-In-Se/ZnS Core/Shell Quantum Dots for In vivo Imaging[END_REF] 164] The lower in vivo toxicity of these alternative material QDs has been examined and experimentally confirmed for CuInS 2 /ZnS and InP/ZnS.[ 164, 166]